We evaluated the filtration performance of microporous metal membranes fabricated by the rolling process. Metal wire meshes were rolled with thickness reduction ratios of 10, 20, and 30%. The pore size of the metal wire mesh membrane decreased with increasing rolling ratio, whereas the removal efficiency of the suspended solids and turbidity showed a very slight increase compared to that of an unrolled mesh membrane. The metal powder was dispersed on the surface of the rolled metal wire mesh membrane and bound with polyvinyl alcohol, then dried at 100°C for 1 h, and finally sintered at 1,000°C for 3 h. The mean pore size, suspended solids, and turbidity of the metal powder membrane at a rolling ratio of 30% were approximately 0.7 μm, 84% and 83%, respectively. Therefore, microporous metal membranes successfully fabricated by the rolling process were also sufficiently permeable filters.
Water conservation and reuse are major issues in groundwater management, desertification, and climate change. Drinking water shortages threaten the survival of the world's population because nearly 50% of the water is used in industry and agriculture (Tang & Chen 2002; Kim et al. 2007; Kujawa et al. 2013).
Porous materials have been used in separation, filtration, absorption, and other chemical processes because of their excellent thermal, acoustic, electrical, and mechanical properties (Liu 2010; Jin et al. 2014). Polymeric membranes are not suitable for use in high concentrations of chlorides, high pH, and high temperature and pressure conditions. Ceramic membranes are brittle if exposed to rapid pressure or temperature variations, whereas metal membranes are not (Rubow et al. 1999; Wang et al. 2004). Metal porous filters are made of sintered metal powders, metal wire mesh, and metal fibers as foundation, can withstand pressures up to 1 MPa and temperatures up to 350°C, and are resistant to oxidation. Metal porous filters have a long lifetime, and this minimizes the maintenance cost. Metal porous filters are sturdy and have constant permeability, high corrosion resistance, and high thermal stability. Consequently, metal membranes have numerous applications in the chemical, electrical and power, environmental, and pharmaceutical industries (Snow et al. 1995; Kim et al. 2005; Herrmann & Morgan 2009).
In this study, we evaluated the fabrication and filtration performance of microporous metal membranes fabricated by the rolling process. Metal wire meshes were rolled with reduction ratios of 10, 20, and 30% (reduction is the decrease in metal thickness). Metal powder membranes were fabricated by dispersing the metal powder on the surface of the rolled metal wire mesh membranes using polyvinyl alcohol (PVA) as binder, then drying at 100°C for 1 h, and finally sintering at 1,000°C for 3 h.
Porous metal wire meshes and metal powder membranes were fabricated by rolling–sintering and dip coating, respectively. Metal wire mesh membranes were prepared using metal meshes #165/1450, #270/2000, and #510/3600. Metal wire mesh (disk-type) of approximately 10 × 10 cm2 was rolled with thickness reduction ratios of 10, 20, and 30%. Then, the five-layer sintered metal mesh membrane was fabricated by rolling and sintering under vacuum (1 × 10−5 Torr) and pressure (10 kgf/cm2) at 1,200°C for 1 h. To fabricate the metal powder membranes, we used SUS 316L metal powder with a mean particle size of 5 μm. Prior to rolling, the metal powder was washed by sonication in ethanol and deionized water and then dried in an oven at 80°C for 2 h. The metal powder was dispersed on the surface of the rolled metal wire mesh membrane (#40/200), using PVA as the binder, dried at 100°C for 1 h, and sintered at 1,000°C for 3 h.
The microstructure of the porous metal membranes was studied by using a Hitachi SU-70 field emission scanning electron microscope (FE-SEM) equipped with an energy dispersive X-ray spectrometer. The mean flow pore diameter (the value for which the flow is decreased almost by half in a partial flow test device) and pore pressure were measured using a capillary flow porometer (PMI, Inc.). The filtration performance of the porous metal membranes was evaluated by measuring the turbidity with a DR/2010 spectrophotometer and the total suspended solids (SS) using Standard Method 2540 (APHA 2005).
RESULTS AND DISCUSSION
Fabrication and filtration performance of the metal mesh membranes
Fabrication and filtration performance of the metal powder membrane
We fabricated porous metal membranes by the rolling process. The structural properties and filtration performance were evaluated by considering SEM images, pore diameter, pore pressure, SS and turbidity. The metal membranes were rolled with a thickness reduction ratio of 10, 20, and 30%. The pore size of the pure metal mesh membrane decreased with increasing rolling ratio, whereas the removal efficiency of SS and turbidity showed a very slight increase compared to that of the unrolled metal mesh membrane. The mean pore size, SS, and turbidity removal of the metal powder membrane with a rolling ratio of 30% were approximately 0.7 μm, 84%, and 83%, respectively. Porous metal membranes were successfully fabricated by the rolling process, and showed adequate filtration performance as membrane filters.
This research was supported by a grant (code 15IFIP-C088924-02) from Industrial Facilities & Infrastructure Research Program funded by the Ministry of Land, Infrastructure and Transport (MOLIT) of the government of Korea.